ferritic stainless steels in structural applications .1 ferritic stainless steels in structural...
Post on 25-Mar-2019
Embed Size (px)
Ferritic stainless steels in structural applications
K.A. Cashell1 and N.R. Baddoo2 1 Department of Civil Engineering, Brunel University, UK 2 The Steel Construction Institute, Ascot, UK
Ferritic stainless steels are low cost, price-stable, corrosion-resistant materials. Although widely used in the automotive and domestic appliance sectors, structural applications are scarce owing to a dearth of performance data and design guidance. The characteristics of ferritics make them appropriate for structures requiring strong and moderately durable structural elements with attractive metallic surface finishes. The present paper provides an overview of the structural behaviour of ferritic stainless steels, including a summary of the findings of a recent European project (SAFSS) on ferritics. Laboratory experiments have been completed including material tests as well as structural member tests, both at ambient and elevated temperature. The experimental data is supplemented by numerical analysis in order to study a wide range of parameters. The findings of this work have enabled design guidance to be proposed, as discussed herein.
Stainless steel is the name given to a family of corrosion and heat resisting steels containing a minimum of 10.5% chromium. Whereas carbon steel needs to be painted with a protective coating if exposed to an outdoor environment, stainless steels have a naturally occurring corrosion resistant surface layer, known as the passive layer, which means that there is no requirement for applying protective surface layers. This invisible passive layer is primarily a consequence of the chromium content of the material.
The use of these materials in load-bearing structural applications has increased in recent years, mainly owing to their favourable strength, stiffness and durability characteristics as well the low maintenance requirements. Stainless steel can be fabricated using a wide range of commonly available engineering techniques, has a high recycled content and is fully recyclable at the end of its service life. It is often specified for structures in aggressive environments such as near deicing salts, water, or heavy pollution as well as in architectural applications. The main drawback is the relatively high initial cost compared with carbon steels although this is often offset over the lifetime of the structure owing to its low maintenance requirements and excellent durability .
There are many different grades of stainless steel meeting a wide range of strength, weldability and durability requirements, and these can be categorised into five groups: austenitic, ferritic, martensitic, duplex and precipitation-hardening grades. The austenitic and duplex grades are most commonly used in structural applications as they provide a good
combination of corrosion resistance, forming and fabrication properties and have been researched and validated. However, there is increased interest in ferritic stainless steels which share many of the attractive properties of austenitic and duplex materials such as strength and durability but are cheaper alloys containing little, or no, nickel. Used in the appropriate applications, ferritics can offer a very competitive and economical solution.
Despite being widely used in the automotive and domestic appliance sectors, structural applications of ferritic stainless steels are scarce owing to a lack of knowledge, performance data and design guidance. They have been specified for cladding and roofing applications as well as in the transportation sector for load-bearing members, for example for tubular bus frames. They have also been used for a range of structural applications in South Africa , including:
1. Structural steelwork for shaft supports in South African gold mines (these deep mines have very aggressive conditions, including high levels of chlorides and temperatures up to 50C).
2. Railway electrification masts along the railway line in Port Elizabeth. The railway line runs along the coast and is constantly exposed to sea spray during windy conditions.
3. Tubular piles and support framework for the Marion Island Weather Station & Research Base, which is situated in a very corrosive environment on a volcanic island 1200 km south-east of Cape Town.
The Eurocode dealing with structural stainless steel, EN 1993-1-4 , states it is applicable to three traditional ferritic grades (1.4003, 1.4016 and 1.4512), however, the guidance is almost exclusively derived from work on austenitic and duplex stainless steels and in many cases ferritic-specific guidance is missing. Even taking into account experience using ferritics in other sectors, until recently there has been insufficient information available on structural performance, fire resistance, atmospheric corrosion resistance and strength of connections to give designers the confidence to specify these materials for structural applications.
It is in this context that a major collaborative project began in Europe in 2010 entitled Structural Applications of Ferritic Stainless Steels (hereafter referred to as SAFSS). The principal aim of the study was to develop the information needed for comprehensive structural design guidance to be included in relevant parts of the Eurocodes and other accompanying standards and guidance. It was also recognised that any limitations of these materials should be acknowledged. Although the research has general applicability to the use of ferritic stainless steel, there is a particular focus on light gauge steel framing, purlins, roof trusses and space-frames structures as well as steel decking for composite floors.
This paper presents a thorough description of ferritic stainless steels including the essential information that is required in order to specify these materials in structural applications. An overview and appraisal of recent research is also provided with the focus given to providing dedicated structural design guidance for the ferritic grades, which is in line with current Eurocode procedures.
2 Ferritic stainless steels
Ferritics are a family of utility stainless steels which offer significantly better atmospheric corrosion resistance than carbon steels, as well as having good ductility, formability and impact resistance. They have been used for a range of applications including vehicle frames/chassis, railway wagons, conveyors, chutes, tanks and walkways in industries such as road and rail transport, water, power generation and mining.
The initial material cost of stainless steel is largely controlled by the alloy content, in particular the level of nickel, which is around 8% - 10% for the common austenitic grades. As ferritic stainless steels do not contain nickel, they are cheaper and relatively price-stable compared with the austenitic grades generally encountered in construction. The cost of austenitics is strongly dependent on the London Metal Exchange (LME) nickel price which is highly volatile and periodically shows dramatic increases (e.g. between 2005 and 2008) thereby distorting the market price for austenitics.
The mechanical and physical properties of ferritic stainless steels, which are described in the current paper, make them suitable for a number of structural applications, for example where strong and moderately durable structural elements with attractive metallic surface finishes are required. Unlike galvanised or painted steel, ferritic stainless steels have a naturally occurring corrosion resistant surface layer so there is no requirement for applying protective surface layers and no remedial work or corrosion risk at cut edges. Ferritic stainless steels can be produced in a range of dull and bright surfaces.
Ferritics generally have limited low-temperature toughness, particularly for thicker sections . The ferritic grade 1.4003, however, has a modified microstructure which ensures adequate toughness for external structural applications (40J at -40C), which is equivalent to structural carbon steel. Ferritics can be welded by conventional methods, though there can be a loss of ductility and toughness. Due to these limitations in low-temperature toughness and weldability, ferritics tend to be used in thicknesses less than 6 mm for thin-walled cold-formed sections (e.g. hollow sections, channels etc.).
Figure 1 illustrates a comparison between the stress-strain responses for a typical ferritic grade with other materials.
2.2 International design standards
Three ferritic grades are covered in the American ASCE/SEI specification for design of cold-formed stainless steel structural members  for thicknesses up to 3.8 mm, namely grades 1.4512, 1.4016 and 1.4510. The South African (South African Bureau of Standards, 1997)  and Australian/New Zealand (Standards Australia Standards New Zealand, 2001)  structural stainless steel standards also include grade 1.4003.
The current version of the Eurocode for structural stainless steel, EN 1993-1-4  states it is applicable to three ferritic grades (Grades 1.4003, 1.4016 and 1.4512), however, the guidance is almost exclusively derived from work on austenitic and duplex stainless steels and in many
cases ferritic-specific guidance is missing. EN 1993-1-4 refers to a number of clauses in other parts of Eurocode 3 such as EN 1993-1-2 , 1-8 , 1-9  and 1-10  which have not been validated for ferritic stainless steels. One exception is that EN 1993-1-2 includes data on one ferritic grade.
The actual corrosion resistance of a particular grade of stainless steel depends on its constituent elements, and hence each grade has a slightly differ